Comparative Evaluation of the Depth of Cure and Degree of Conversion of Two Bulk Fill Flowable Composites
CA Anand Yokesh1, P Hemalatha2, M Muthalagu3, M Robert Justin4
ABSTRACT Introduction: Since the development of resin based composites, several improvements have been made to improve their physical and chemical properties. In an attempt to fasten and simplify the restoration process, a new class of resin based composite materials, called the bulk fill resin based composites have been introduced, which has been claimed to achieve a depth of cure of 4 mm without affecting the properties of the material. Aim: To comparatively evaluate the depth of cure of two different bulk fill flowable composite resins by ISO 4049 method and to evaluate the degree of conversion of the same composite resins with Fourier Transform Infrared (FTIR) spectroscopy method. Materials and Methods: Composite resin specimens (n=10) per group were prepared with bulk fill flowable composites, Surefil SDR flow (Dentsply Caulk, Milford, DE, USA) designated as Group A and Filtek bulk fill (3M ESPE, St.Paul, MN, USA) designated as Group B. Depth of cure was determined according to “ISO 4049; Depth of Cure” method, and FTIR spectroscopy method
was used to estimate the degree of conversion of both the bulk fill flowable composites. The degree of conversion of monomer to polymer was estimated individually in coronal half (Group A1 and B1) and pulpal half (Group A2 and Group B2) by dividing each specimens into two halves. The data were analysed using Student’s unpaired t-test at 5% level of significance. Results: The mean depth of cure of Group A was 3.89 mm (±0.103) and for Group B was 3.54 mm (±0.129). The degree of conversion percentage for Group A1=78.51 (±47.8), Group A2= 31.9 (±22.4), Group B1=39.8 (±5.2), Group B2=37.4 (±6.4). Statistical analysis revealed significant difference in the depth of cure between the two bulk fill flowable composites with Group A higher than Group B. The degree of conversion of the coronal half of Group A1 was significantly higher when compared to Group B1. Conclusion: Surefil SDR bulk fill resin has better depth of cure and degree of conversion compared to Filtek bulk fill composites.
Keywords: Carbon-carbon double bond conversion, Composite resin, Degree of polymerization, Fourier transform infrared spectroscopy
Introduction The clinical success of resin composite restoration depends on various parameters like depth of cure, degree of polymerization, polymerization shrinkage, linear coefficient of thermal expansion, modulus of elasticity, wear resistance, C-factor etc. Depth of cure is defined as the thickness of a light cured resin that can be converted from a monomer to a polymer when exposed to a light source under a specific set of conditions . Degree of conversion is defined as the percentage of carbon-carbon double bonds (- C = C -) converted to single bonds (- C - C -) to form a polymeric resin . When light is transmitted through the composite resin, there is a gradual decrease in degree of conversion as the distance increases from the irradiated surface which leads to elution of monomer causing failure of the restoration [2-5]. Increment thickness of 2 mm is the gold standard for composite placement and curing [6,7]. It is highly technique sensitive and time consuming in cases of larger posterior restorations or during core build up procedures, where composite restorations are indicated. To address these problems, various manufactures have recently introduced new type of resins, so called “bulk fill” materials which claim to cure a maximum increment thickness of 4 mm [8-11]. There are some relevant methods to determine the degree of monomer to polymer conversion of composite resin specimens like FTIR spectroscopy, Laser Raman spectroscopy, Electron Spin Resonance (ESR), Infrared Spectroscopy (IR), Dynamic Mechanical Thermal Analysis (DMTA), Attenuated Total Reflection (ATR) etc., . Of these, the most reliable method to determine the extent 86
of monomer conversion is FTIR, which can detect the stretching vibrations of carbon-carbon double bonds involved in polymerization directly before and after curing of the composite resins [13-15]. The method typically utilizes the height ratio of the peaks corresponding to aliphatic and aromatic double bonds to determine the degree of conversion. A method for finding the curing of the maximal increment thickness of resin composites has been introduced by the International Organization for Standardization (ISO) in the second edition of ISO 4049. In 1988, it was officially denominated as “ISO 4049, Depth of Cure” . According to this method, a teflon mold was used to create the composite specimen. The specimens were removed from the mold after light curing and uncured resin was scraped off with a plastic instrument. The length was measured and divided by 2 as per ISO 4049 method . Hence, the aim of this study was to comparatively evaluate the depth of cure of two different bulk fill composite resins (Surefil SDR bulk fill flowable and Filtek bulk fill flowable composite) by ISO 4049 method and to evaluate the degree of conversion of the same composite resins with FTIR spectroscopy method. The tested null hypothesis was that there is no difference in depth of cure and degree of conversion between the two bulk fill flowable composite materials.
MATERIALS AND METHODS This in vitro study was conducted in Department of Conservative Dentistry and Endodontics at Best Dental Science College and Dental Hospital, Madurai, Tamil Nadu, India, after getting approval Journal of Clinical and Diagnostic Research. 2017 Aug, Vol-11(8): ZC86-ZC89
CA Anand Yokesh et al., Evaluation of Two Bulk Fill Composites
of the Ethical committee. Based on the figures of bottom hardness reported in previous study , the sample size for this study was calculated as 10 samples per group for a confidence level of 95% and a power of 95%. Hence, composite resin specimens (n=10) per group were prepared with both bulk fill flowable composites, Surefil SDR bulk fill flowable composite (Dentsply Caulk, Milford, DE, USA) designated as Group
After determining the depth of cure of resin composite specimens, each specimen in Group A and Group B, which were of different sizes were divided into two equal halves. They were referred as coronal half and pulpal half, designated as Group A1, A2 and Group B1, B2 respectively. Hence, 20 specimens per each group and total of 40 resin composite specimens were made to estimate the degree of monomer to polymer conversion individually in coronal half (Group A1 and B1) and pulpal half (Group A2 and Group B2). All specimens were pulverized and mixed with potassium bromide (KBr) in 1:10 ratio as it is 100% transparent with wide spectral range. The specimens were then pressed in hydraulic pellet maker (Pixie hydraulic pellet press, Pike technologies, Madison, USA) which is thin, transparent and 13 mm in diameter. The prepared pellets were placed into a cell holder in spectrophotometer and the readings were made [Table/Fig-4]. Degree of Conversion is calculated by the formula ,
H2 peak height absorbance intensity of carbon double bond peak aliphatic [Table/Fig-1]: Group A and Group B Surefil SDR bulk fill flowable composite and Filtek Bulk fill flowable fill flowable composite.
A and Filtek bulk fill flowable composite (3M ESPE, St.Paul, MN, USA) designated as Group B [Table/Fig-1,2].
Estimation of Depth of Cure Depth of cure was determined according to “ISO 4049; Depth of Cure” method, using re-usable teflon mold of 8 mm length and 4 mm diameter. The mold was placed on a glass slide covered by a mylar strip and then the teflon mold was filled in bulk with one of the bulk fill flowable composites. The top side of the mold was covered with a mylar strip and light cured for 20 seconds, keeping the light tip centered and in contact with the material (LEDition, Ivoclar Vivadent AG, Schaan, Liechtenstein, operating at 7.5 VDC, 3W LED, with a wavelength range of 430-490 nm and typical light output of 600 mW/cm2). After light curing, the cylindrical specimens were pushed out of the teflon mold and the uncured resin composite material was removed or scrapped off with a plastic spatula. This technique gave specimens of different sizes. The absolute length of the cylindrical specimen of the cured resin composite was then measured with a digital caliper of ±0.01 mm accuracy [Table/Fig-3]. The absolute length was divided by two and the value was recorded as ‘Depth of Cure’. The same procedure was repeated for estimating the depth of cure for all the specimens. Hence, the procedure was done ten times for each group to obtain ten specimens per group.
Estimation of Degree of Conversion The degree of conversion of both bulk fill flowable composites (Surefil SDR and Filtek flowable bulk fill composites) was estimated using FTIR method. Group
H1 peak height absorbance intensity of carbon double bond peak aromatic.
Statistical analysis Statistical analysis was performed by Statistical Package for Social Sciences (SPSS Inc., Chicago, IL, version 19.0 for Windows). Using this software mean and standard deviation were calculated for quantitative variables. Student’s unpaired t-test was used to test the significance of difference between the two groups. A p-value of less than 0.05 is taken to denote the significant relationship.
RESULTS Depth of Cure The mean depth of cure of Group A (Surefil SDR bulk fill flowable composites) was 3.89 mm (±0.103) and for Group B (Filtek bulk fill flowable composites) was 3.54 mm (±0.129) [Table/Fig-5]. Statistical analysis revealed significant difference (p